Primer is the most important step in the construction process of epoxy floor paint. Only when this step is completed can the next coating be continued on the base surface. Therefore, the general requirements for primers used in floor coating are: good adhesion with the substrate; good mechanical strength; good protection against the substrate and no adverse side effects; can create a good foundation for future coatings, can not contain the components of the defects caused by infiltration into the upper coating; Better construction and dryness.
Primer coating should generally pay attention to the surface treatment in strict accordance with the prescribed time and timely coating primer. A paint should also be applied within the time limit specified after the primer is dried according to the conditions stipulated in the primer. Early coating may cause underbite and difficulty in solvent evaporation in primer resulting in prolonged drying time `poor solidification, bubbling and other conditions; late coating may cause poor adhesion between layers, and late coating is easy to affect the apparent quality due to dust accumulation or other pollution. To increase adhesion between the next coating and primer, the primer can be ground before coating.
Coating primers are generally made by roller coating, brush coating and spraying. Brush construction efficiency is low, usually in the corner construction. The most commonly used roller coating is highly efficient. 封閉底漆施工：
Construction of closed primer:
Use brush, roll or spray to apply one or two closed floor primers. The interval between the two primers is more than 8 hours, but not more than 48 hours. For old ground, a primer should be added. Attention should be paid to uniform coating when priming is applied, and no obvious difference in thickness is observed to prevent leakage. Attention should be paid to the accumulation of residual materials by roller coating method. When the primer is not fully sealed (leak coating), it will cause adhesion, coating and bubbling.
1. primer paint film thickness should be determined according to primer varieties, and attention should be paid to control. There is no floating dust and loose sand on the surface.
2. primer with pigments and fillers should be evenly stirred before use and during use.
3. pay attention to the drying specifications. Primers must be dry when priming is applied to paints containing strong solvents, so as to avoid biting diseases.
4. increase the adhesion between the next coating and primer, so that the primer can be ground before coating.
5. before coating the surface, the primers should be coated in strict accordance with the prescribed time. A paint should also be applied within the specified time limit after the primer is dried according to the conditions stipulated in the primer. Early coating may cause priming and solvent evaporation difficulties in primers lead to prolonged drying time and poor solidification of the film; too late coating may lead to poor adhesion between layers, and too late coating may easily be affected by dust accumulation or other pollution.
Primer dilution according to the instructions and epoxy resin floor paint construction needs, control the proportion, prohibit excessive dilution.
The ground must be cleaned when the base is fully dry and there is no foreign matter. If the ground does not meet the requirements, it should be reported to the project manager in time.
When the epoxy floor paint is opened, it should be fully stirred and used again.
First brush the edges and corners and the parts which are not easy to stick, and then carry out large-scale construction from top to bottom, not easy to absorb material for the floor with brush point brush epoxy resin floor paint primer.
When painting, the barrel must be equipped with rollers, sticks and brushes dipped in the material must be on the rollers after licking material can be constructed.
If brush hair or club hair is stained on the wall, it should be dealt with promptly.
Due to the rapid volatilization of solvents, if the thickening of the primer during construction affects the construction, the appropriate amount of solvents can be added, but in general, this method is not recommended.
Check if there is any leakage on the ground and repair it.
The repainting time is usually greater than 6-8 hours.
Epoxy floor paint construction effect coating rate to meet the requirements; do not allow the phenomenon of leakage coating and flow, obvious rubbing, to achieve uniform stick coating. If there is a big difference between the actual coating rate and the coating rate, it should be reported to the project manager.
In the construction of epoxy floor paint, primer is a crucial point. Only when the base surface is sealed, can the next coating be carried out. If the primer is not done well, even if the later process is done well, it will be lost.
Other aspects should be noted:
For pits in cement base, fill them with commercial epoxy putty or epoxy mortar with primer and fine quartz sand, and then grind them smoothly after solidification.
Middle level coating construction:
For thick film coatings, trowel trowel can be used in middle coating construction. Due to the use of more quartz sand in the paint, the film will not appear obvious scratch marks under normal circumstances, but if the addition of quartz sand is too large, scratch obvious should be rolled once. If the coating interval is greater than 48 hours, the next coating should be applied after grinding to ensure interlaminar adhesion.
Surface coating construction:
According to the types of epoxy abrasion resistant floor coatings, the surface coating can be constructed by brush or scraping. For thick film coatings, mix the two components evenly according to the proportion requirements, and use 1mm scraper coating after curing. During scraping, thick film should be kept as uniform as possible without any leakage. When scraping, the moving speed of the scraper should be uniform, and the angle between the scraper and the ground plane should be about 30 degrees to ensure the film thickness. The number of scraper passes depends on the thickness requirements. Ordinary epoxy coatings can be constructed by brush method. The interval between the two surfaces should be above 18h, but not more than 48h. The coatings should be used up as soon as possible to prevent the viscosity of the coatings from rising and the bubbles in the coatings are difficult to discharge.
Epoxy floor maintenance:
After the surface coating has been applied and completely cured, it should be applied for more than 24 hours before it can be applied, and 72 hours after it can be repressed. (at 25 C, the opening time at low temperature should be extended moderately). 本站網址：http://www.msxgb.com